# solution set 6 ```Core 8.15
The values might not be correct.
6.7
For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and
the modulus of elasticity is 115 GPa (16.7 &times; 106 psi).
(a) What is the maximum load that may be applied to a specimen with a cross-sectional area of
325 mm2 (0.5 in.2) without plastic deformation?
(b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to which it
may be stretched without causing plastic deformation?
Solution
(a) This portion of the problem calls for a determination of the maximum load that can be
applied without plastic deformation (Fy). Taking the yield strength to be 275 MPa, and employment
Fy = σ y A0 = (275 &times; 10 6 N/m 2 )(325 &times; 10 -6 m 2 )
= 89,375 N
(20,000 lbf)
(b) The maximum length to which the sample may be deformed without plastic deformation is
determined from Equations 6.2 and 6.5 as
⎛
σ⎞
li = l0 ⎜1 + ⎟
⎝
E⎠
⎡
275 MPa ⎤
= (115 mm) ⎢1 +
⎥ = 115.28 mm (4.51 in.)
115 &times; 10 3 MPa ⎦
⎣
6.10 Consider a cylindrical specimen of a steel alloy (Figure 6.21) 10.0 mm (0.39 in.) in diameter
and 75 mm (3.0 in.) long that is pulled in tension. Determine its elongation when a load of 20,000 N
(4,500 lbf) is applied.
Solution
This problem asks that we calculate the elongation ∆l of a specimen of steel the stress-strain
behavior of which is shown in Figure 6.21. First it becomes necessary to compute the stress when a
load of 20,000 N is applied using Equation 6.1 as
σ =
F
=
A0
F
⎛d ⎞
π⎜ 0 ⎟
⎝2⎠
2
=
20, 000 N
⎛ 10.0 &times; 10−3 m ⎞2
π⎜
⎟
2
⎝
⎠
= 255 MPa (37,700 psi)
Referring to Figure 6.21, at this stress level we are in the elastic region on the stress-strain curve, which
corresponds to a strain of 0.0012. Now, utilization of Equation 6.2 to compute the value of Δl
Δ l = ε l0 = (0.0012)(75 mm) = 0.090 mm (0.0036 in.)
6.13 In Section 2.6 it was noted that the net bonding energy EN between two isolated positive and
negative ions is a function of interionic distance r as follows:
EN = −
A B
+
r rn
where A, B, and n are constants for the particular ion pair. Equation 6.25 is also valid for the bonding
energy between adjacent ions in solid materials. The modulus of elasticity E is proportional to the
slope of the interionic force–separation curve at the equilibrium interionic separation; that is,
⎛ dF ⎞
E ∝⎜ ⎟
⎝ dr ⎠r
o
Derive an expression for the dependence of the modulus of elasticity on these A, B, and n parameters
(for the two-ion system) using the following procedure:
1. Establish a relationship for the force F as a function of r, realizing that
F=
dEN
dr
2. Now take the derivative dF/dr.
3. Develop an expression for r0, the equilibrium separation. Since r0 corresponds to the value of r
at the minimum of the EN-versus-r curve (Figure 2.8b), take the derivative dEN/dr, set it equal to zero,
and solve for r, which corresponds to r0.
4. Finally, substitute this expression for r0 into the relationship obtained by taking dF/dr.
Solution
This problem asks that we derive an expression for the dependence of the modulus of elasticity, E,
on the parameters A, B, and n in Equation 6.25. It is first necessary to take dEN/dr in order to obtain
an expression for the force F; this is accomplished as follows:
⎛B⎞
⎛ A⎞
d⎜ ⎟
d ⎜− ⎟
dE N
⎝ r⎠
⎝rn ⎠
F =
=
+
dr
dr
dr
=
A
r2
−
nB
r (n +1)
(6.25)
The second step is to set this dEN/dr expression equal to zero and then solve for r (= r0). The algebra
for this procedure is carried out in Problem 2.14, with the result that
⎛ A ⎞1/(1 − n)
r0 = ⎜ ⎟
⎝ nB ⎠
Next it becomes necessary to take the derivative of the force (dF/dr), which is accomplished as
follows:
⎛ A⎞
⎛
nB ⎞
d⎜ ⎟
d ⎜−
⎟
dF
⎝r2 ⎠
⎝ r (n +1) ⎠
=
+
dr
dr
dr
=−
2A
r3
+
(n)(n + 1)B
r (n + 2)
Now, substitution of the above expression for r0 into this equation yields
⎛ dF ⎞
2A
(n)(n + 1) B
+
⎜ ⎟ =−
3/(1−
n)
⎝ dr ⎠r
⎛ A⎞
⎛ A ⎞(n + 2) /(1− n)
0
⎜ ⎟
⎜ ⎟
⎝ nB ⎠
⎝ nB ⎠
which is the expression to which the modulus of elasticity is proportional.
6.14 Using the solution to Problem 6.13, rank the magnitudes of the moduli of elasticity for the
following hypothetical X, Y, and Z materials from the greatest to the least. The appropriate A, B, and n
parameters (Equation 6.25) for these three materials are tabulated below; they yield EN in units of
electron volts and r in nanometers:
Material
A
B
X
2.5
2.0 &times; 10–5
2.3
–6
10.5
–5
9
Y
Z
n
8
8.0 &times; 10
3.0
1.5 &times; 10
Solution
This problem asks that we rank the magnitudes of the moduli of elasticity of the three
hypothetical metals X, Y, and Z. From Problem 6.13, it was shown for materials in which the
bonding energy is dependent on the interatomic distance r according to Equation 6.25, that the modulus
of elasticity E is proportional to
E ∝−
2A
⎞3/(1− n)
⎛ A
⎜ ⎟
⎝ nB ⎠
(n)(n + 1) B
+
⎛ A ⎞(n + 2) /(1− n)
⎜ ⎟
⎝ nB ⎠
For metal X, A = 2.5, B = 2.0 &times; 10-5, and n = 8. Therefore,
E ∝ −
(8)(8 + 1) (2 &times; 10−5 )
+
⎡
⎤ 3/(1 − 8)
⎡
⎤(8 + 2) /(1 − 8)
2.5
2.5
⎢
⎥
⎢
⎥
⎢ (8) (2 &times; 10−5 ) ⎥
⎣ (8) (2 &times; 10−5 ) ⎦
⎣
⎦
(2)(2.5)
= 1097
For metal Y, A = 2.3, B = 8 &times; 10-6, and n = 10.5. Hence
E ∝ −
(2)(2.3)
⎡
⎢
⎢ (10.5)
⎣
2.3
(8 &times;
⎤ 3/(1 − 10.5)
⎥
10−6 ⎥⎦
)
+
(10.5)(10.5 + 1) (8 &times; 10−6 )
⎡
⎤(10.5 + 2) /(1 − 10.5)
2.3
⎢
⎥
⎣ (10.5) (8 &times; 10−6 ) ⎦
= 551
And, for metal Z, A = 3.0, B = 1.5 &times; 10-5, and n = 9. Thus
E ∝ −
(9)(9 + 1) (1.5 &times; 10−5 )
+
⎡
⎤ 3/(1 − 9)
⎡
⎤(9 + 2) /(1 − 9)
3.0
3.0
⎢
⎥
⎢
⎥
⎢ (9) (1.5 &times; 10−5 ) ⎥
⎣ (9) (1.5 &times; 10−5 ) ⎦
⎣
⎦
(2)(3.0)
= 1024
Therefore, metal X has the highest modulus of elasticity.
6.D1 A large tower is to be supported by a series of steel wires. It is estimated that the load on each
wire will be 11,100 N (2500 lbf). Determine the minimum required wire diameter assuming a factor
of safety of 2 and a yield strength of 1030 MPa (150,000 psi).
Solution
For this problem the working stress is computed using Equation 6.24 with N = 2, as
σw =
σy
2
=
1030 MPa
= 515 MPa (75,000 psi )
2
Since the force is given, the area may be determined from Equation 6.1, and subsequently the original
diameter d0 may be calculated as
A0 =
⎛ d ⎞2
F
= π⎜ 0 ⎟
σw
⎝ 2 ⎠
And
d0 =
4F
=
π σw
(4)(11,100 N)
π (515 &times; 10 6 N / m2 )
= 5.23 &times; 10-3 m = 5.23 mm (0.206 in.)
7.1 To provide some perspective on the dimensions of atomic defects, consider a metal specimen that
has a dislocation density of 104 mm-2. Suppose that all the dislocations in 1000 mm3 (1 cm3) were
somehow removed and linked end to end. How far (in miles) would this chain extend? Now suppose
that the density is increased to 1010 mm-2 by cold working. What would be the chain length of
dislocations in 1000 mm3 of material?
Solution
The dislocation density is just the total dislocation length per unit volume of material (in this case
per cubic millimeters). Thus, the total length in 1000 mm3 of material having a density of 104 mm-2
is just
(10 4 mm-2 )(1000
mm3) = 10 7 mm = 10 4 m = 6.2 mi
Similarly, for a dislocation density of 1010 mm-2, the total length is
(1010 mm-2 )(1000
mm3 ) = 1013 mm = 1010 m = 6.2 &times; 10 6 mi
7.20 Briefly explain why small-angle grain boundaries are not as effective in interfering with the slip
process as are high-angle grain boundaries.
Solution
Small-angle grain boundaries are not as effective in interfering with the slip process as are
high-angle grain boundaries because there is not as much crystallographic misalignment in the grain
boundary region for small-angle, and therefore not as much change in slip direction.
12．
B
```